Synthesis of different types of nano-hydroxyapatites for efficient photocatalytic degradation of textile dye (Congo red): a crystallographic characterization

The textile industry, a vital economic force in developing nations, faces significant challenges including the release of undesired dye effluents, posing potential health and environmental risks which need to be minimized with the aid of sustainable materials. This study focuses on the photocatalytic potential of hydroxyapatite together with different dopants like titanium-di-oxide (TiO2) and zinc oxide (ZnO). Here, we synthesized hydroxyapatite (HAp) using different calcium sources (calcium hydroxide, calcium carbonate) and phosphorous sources (phosphoric acid, diammonium hydrogen phosphate) precursors through a wet chemical precipitation technique. Pure and doped HAp were characterized via different technologies, which consist of X-ray diffraction (XRD), Fourier Transform Infrared (FTIR) spectroscopy, scanning electron microscopy (SEM), as well as UV-vis spectroscopy. The effectiveness of the synthesized photocatalyst was evaluated by its interactivity with synthetic azo dyes (Congo red). The photodegradation of Ca(OH)2_HAp, CaCO3_HAp, ZnO-doped HAp as well as TiO2-doped HAp, were obtained as 89%, 91%, 86%, and 91%, respectively. Furthermore, at neutral pH, TiO2-doped HAp shows the highest degradation (86%), whereas ZnO-doped HAp possesses the lowest degradation (73%). Additionally, various XRD models (Monshi–Scherrer's, Williamson–Hall, and Halder–Wagner methods) were employed to study crystallite dimension.


Introduction
Water pollution and the energy crisis are being addressed as global headaches and becoming more crucial events via population growth and fast industrialization.The worldwide production of organic dyes is approximately 450 000 tons, whereas 20-60% of wastewater is generated using hazardous organic azo dyes by numerous industries like pigment, fertilizer, cosmetics, paper, and textile. 1,2Synthetic dyes like Congo red (CR) are tough to biodegrade because of their stable molecules as well as complicated aromatic structures, which might induce carcinogenic and mutagenic effects. 3,4Several purication processes, such as reverse osmosis ltration, biological degradation, adsorption, occulation, and centrifugation, were developed for wastewater purication. 5,6However, the majority of these purication techniques are plucked entirely for the degradation of the organic dye, owing to their high expenditure in operation, complex steps, and difficulty in applications. 7So, there is an urgent necessity to develop the existing technique that makes the purication process more efficient, easier, economical, and eco-friendly for synthetic dye degradation.Considering the above-mentioned criteria, the photocatalytic phenomena became a prominent innovation for the deterioration of synthetic dye along with various inorganic compounds like phenol and their derivatives. 8,9However, the degradation efficiency of dyes depends on the nature of the photocatalyst used.Because of this, several photocatalysts have been developed to estimate their performance in synthetic dye degradation. 10,113][14] Ideal HAp [Ca 10 (-PO 4 ) 6 (OH) 2 ] crystal is monoclinic in nature.However, conventional HAp has a lattice deciency, which consists of a hexagonal ionic compound along with a P6 3 /m space group, as well as 44 atoms in every repeating unit.The cations "Ca" are separate two distinctive sites such as Ca(I) and Ca(II).Ca(I) is associated with the columnar site along with the c axis, where Ca(II) is located around OH ions. 15Since HAp has a complex molecular arrangement, various types of cations can be incorporated into its crystal structure.][18][19] Titanium dioxide (TiO 2 ) and zinc oxide (ZnO), along with other semiconductors, have lately been used as affordable and environmentally safe photocatalysts for the decomposition of different contaminants. 20Conversely, ZnO has a signicant advantage over TiO 2 in terms of its ability to absorb a larger portion of the UV spectrum. 213][24] Though HAps are well known bioceramics, these can be utilized as the photocatalytic materials.HAp in pure form cannot impart so much catalytic activity but in doped form or with the combination other materials the photocatalytic activity is increased.Normally metals are used to replace the calcium ions of hexagonal crystal of HAp.
In this present work, HAp was synthesized from CaCO 3 and Ca(OH) 2 by wet chemical precipitation method.TiO 2 and ZnO were used to replace the calcium ions to modify the crystallographic parameter with a hope to augment the photocatalytic activity.In-depth crystallographic analysis was also performed to nd out the variation due to doping the materials.

Materials
To proceed with this experiment, calcium carbonate (CaCO 3 ) and calcium hydroxide (Ca(OH) 2 ), as well as phosphoric acid (H 3 PO 4 ), are utilized as potential sources for calcium and phosphate correspondingly.Apart from that, zinc oxide (ZnO), along with anhydrous titanium dioxide (TiO 2 ), is employed as a dopant for synthesizing doped Hydroxyapatite.All these chemicals were purchased from E-Merck, Germany.No buffer solution was utilized in this experiment, but ammonium hydroxide (NH 4 OH) and nitric acid (HNO 3 ) were used to maintain the pH (10-11) of the reaction media.The production of deionized (DI) water was simplied via a two-stage distillation procedure.

Synthesis of doped and pure HAp.
To synthesize pure and metal-oxide doped HAp, the molar ratio of calcium and phosphate was maintained as 5 : 3.At the beginning, a predetermined amount of Ca 2+ , as well as TiO 2 (0.05%) and ZnO (0.05%), are separately dissolved in 50 mL DI.Diammonium hydrogen phosphate [(NH 4 ) 2 HPO 4 ] and H 3 PO 4 were then added into the different Ca 2+ solutions [CaCO 3 and Ca(OH) 2 ] at the rate of 4 mL min −1 .The solution is then stirred at 300 rpm while introducing H 3 PO 4 and [(NH 4 ) 2 HPO 4 ] into the calciumcontaining solution.Furthermore, the pH of the system was controlled at 10-11 by employing a 30% NH 4 OH solution.Finally, the solution was ltered and dried at 105 °C.A similar approach was conducted for metal-oxide-doped HAp (Fig. 1).
2.2.2 Photocatalytic activity.The photocatalytic activity of pure and doped HAp was observed for the deterioration of Congo red dye (CR) solution under a halogen lamp (SEN TAI JM-500), which is placed on the top of the in-house built wooden box shown in Fig. 2. The distance from the lamp to the CR solution was kept constant (0.14 m).The box is then introduced into the cooling water circulation system.Additionally, the temperature and humidity of this system were maintained at approximately ∼25 °C and 60%, respectively.UV-vis spectrophotometer (Hitachi U-2910) was utilized to measure the absorbance of the dye solution by utilizing concentration.The degradation percentage (D p ) as well as degradation capacity (q e ) were measured by employing mathematical eqn (a) and (b).

Degradation percentage :
Degradation capacity : Here, C t and C 0 denote the nal as well as initial concentration of the samples at time "t" correspondingly. 25In comparison, V and W represent the volume of the dye solution and the weight of the catalyst correspondingly.2.2.3 Scavenger's experiment.The captured test for radicals, and electrons was performed to examine the nest suitable species connecting photodegradation of dye under simulated sunlight (i.e.halogen lamp).Several scavengers were used in principal component analysis to measure the function of hydroxyl radicals, holes, and electrons. 26Using the abovementioned ideal setting, isopropyl alcohol (IPA) as well as ethylenediaminetetraacetic acid (EDTA) were utilized to examine the function of hydroxyl radicals and electrons on all synthesized Hap.If not mentioned otherwise, 10 mL of the scavenger was chosen in 40 mL of 20 ppm Congo red dye for 90 min using 0.1 g of catalyst.3 Results and discussion

XRD data interpretation
The patterns, obtained from XRD for doped HAp as well as pure HAp are exhibited in Fig. 3.The plane positions for these samples were visible at (002) The crystallographic study assesses crystalline features such as cell volume, degree of crystallinity, dislocation density, lattice parameters, crystallinity index, microstrain, and crystallite size, employing eqn (1)- (7). 27,28ttice parameter equation; In the previously mentioned formulas, the unit cell is indicated by plane (h,k,l) and a,b,c reects as lattice variable, X c = crystallinity degree, q = angles of the diffraction (in degree), b = FWHM (full width at half maximum) in radian, D c = dimension of repeating unit, d = dislocation density, K = shape factor (arbitrary constant)/Scherrer's constant = 0.94, H (hkl) = peak height of the respective plane, K a = 0.24, for HAp, as well as CI XRD = crystallinity index.The specic surface area of the synthesized HAp was estimated through eqn (8).Where density as well as crystallite dimensions of HAp were denoted by r (3.16 g cm −3 ) as well as D c . 29ecific surface area; Crystallite dimensions in orderly distributed substances are essential in different uses, alongside minuscule crystallites being distinguished by enormous surface areas and vice versa. 30icrostrain leads to crystallite deformation, which results in changes in element's features, especially applicability.Imperfection in crystalline substances is brought about by defects such as point dislocation, line dislocation, and area dislocation, which have a strong connection to the structure of the crystal. 31he value of line dislocation was determined via eqn (6), and the date is shown in Table 1.
The level of crystallinity signicantly impacts the properties of materials, yet efficiently modulating it can be challenging.The investigation indicates that HAp exhibits levels that vary in the degree of crystallinity, while microstrain alludes to the intrinsic stress of crystalline planes, which can manifest as tensile or compressive forces.
The crystallinity index (CI) is explained for measuring the numerical quantication of crystal structure.In this segment, solely the (XRD) X-ray diffraction data were analyzed for calculating the crystallinity index by utilizing eqn (7), and the resulting values are shown in Table 1.
3.1.1Estimation of crystallite size using various models.Exact crystallite dimension estimation for any purpose is a vital requirement.Yet, for determining the size of the crystallite of  HAp specimens, many approaches and algorithms have been developed, including the Williamson-Hall Method (WHM), Monshi-Scherrer Method (MSM), and Halder-Wagner Method (HWM).The Williamson-Hall Method was also expanded, focusing on the UDEDM (uniform deformation energy density model), UDM (uniform deformation model), and UDSM (uniform stress deformation model).

Monshi-Scherrer method (MSM).
To measure the precise size of the crystal, Monshi-Scherrer's method, which is also known as the modied form of Scherrer's equation, is utilized.This revised equation was developed by taking "ln" on the side of Scherrer's equation, which is denoted in eqn (3).The mathematical formula of this modied form is expressed in eqn (9). 32 For the implementation of the graph of this revised model, ln 1 cos q was placed on the X-axis, and ln b was evaluated on the Y-axis (shown in Fig. 4).The straight-line equation (y = mx + c) and the eqn (9) were analyzed to estimate the slope, where the intercept was noted as Kl D MÀS .This method supplied an indicator for the assessment of the reliability of results.Subsequently, the resultant magnitude of crystal size was obtained 5.96 nm for Ca(OH) 2 _HAp, 9.29 nm for TiO 2 _HAp, 103.56 nm for CaCO 3 _-HAp, and 7.12 nm for ZnO_HAp.

Williamson-Hall method (WHM).
Scherrer's Equation, whereas resolving the impact of the Size of crystallite on XRD reection, neglects the inherent strain in nanocrystals resulting from factors like dislocations, point defects, stacking, as well as boundaries of grains. 33The Williamson-Hall examination may identify an inherent strain, which can be determined by examining the effect of strain on crystallite dimension data.Eventually, the overall broadening may be described as eqn (10). 34Total = b size + b strain (10)   where b strain is connected to the strain broadening effect as well as b size is the broadening due to its size.The modied form of the Williamson-Hall, considered a UDM, USDM, and UDEDM, will be discussed in this context.35 3.1.4Uniform deformation model (UDM).The estimated value of strain derived through crystalline defects and deformation in the synthetic HAp can be mathematically represented as a eqn (11).36 3 ¼ b hkl 4 tan q (11) The UDM idea relies on the concept of homogenous strain in all directions and regards lattice strain as isotropic in nature despite its spatial amplitude. 37The peak broadening, which is caused via lattice strain, is oen denoted in eqn (12).
The overall broadening, b hkl is expressed as FWHM of a re-ected peak, which is related to the inuence of the strain of crystal lattice (b strain ) and the value of the size of the crystals (b size ) in a specic peak that may be stated as eqn ( 13)- (15).
Eqn ( 14) can be written as:  b hkl cos q ¼ Placing 4 × sin q along the X-axis as well as b hkl × cos q on the Y-axis permits a straight-line equation.In the graph, both slope (3) and crystallite size (D w ) (y-intercept) can be computed.The graphs are depicted in Fig. 5, and the computed (D w ) and 3 values are reported in Table 2.
3.1.5Uniform stress deformation model (USDM).UDM models, depending on material homogeneity and isotropic nature, frequently remain unvalidated because of the potential anisotropic nature of real crystals, requiring an altered Uniform Stress Deformation Model (USDM). 33From Hooke's law, it is known that there is a linear link between 3 (Strain) as well as stress (s) expressed via eqn (16).
The mathematical expression Y hkl depicts Young's modulus or modulus of elasticity, which is a reliable approximation for minimal strain.Increasing the amount of strain causes a shi in the magnitude of Young's modulus, demonstrating that the strain is not linear in nature. 38By rearranging and replacing eqn (16) with eqn (10), we have the following relation (eqn (17)) Thus, plotting b total × cos q on the Y-axis as well as 4 × sin q/ Y (hkl) along the X-axis produces a straight-line graph.The gradient of this expressed straight line delivers a measure of stress (s), whilst the point of intersection offers the crystallite size D (hkl) of the HAp nanocrystals.The plots are illustrated in Fig. 6, and the computed s and D (hkl) values are shown in Table 2.
3.1.6Uniform deformation energy density model (UDEDM).UDM includes anisotropic entities that necessitate an alteration of the W-H relationship for effective alignment in

Model name
Crystallite size (in nm), strain, anisotropic nanocrystals. 39UDEDM, determined by Hooke's law, demonstrates a linear relationship between s and 3 in real crystals.Yet, this straight proportionality is unsuitable since there are defects in the long-range order, including agglomerations and dislocations.UDEDM evaluates crystal imperfections, asymmetric deformation, and distortion causes as a measure of energy density (u), so the stress and strain constants remain independent. 40Eqn (18) denotes 3 (energy per unit volume), which is determined by Hooke's expression.
By plotting the graph between b total cos q on the Y-axis as well as 4 sin q ffiffiffi 2 p ffiffiffiffiffiffiffi ffi Y hkl p .On the X-axis, an anisotropic energy density (u) and crystallite size (D w ) were measured from the slope and Yintercept (Fig. 7).The estimated crystallite dimensions are shown in Table 2.
3.1.7Halder-Wagner method (HWM).The SSP technique utilizes the Gaussian function to express the expansion of tension and the Lorentzian function to symbolize the broadening of size in XRD patterns.However, the XRD area correlates to the Gaussian operation, whereas the bottom drops excessively.The lower portion of the prole ts the Lorentz function yet does not match the XRD peak area. 41,42The Halder-Wagner approach employs the symmetrical Voigt function, a convolution of Gaussian and Lorentzian processes, to describe the FWHM of the physical prole, as illustrated in eqn (20).
A plot of (*b hkl /*d hkl ) 2 on the Y-axis and *b hkl /(*d hkl ) 2 on the Xaxis generates a straight line, where slope equal to 1/D w and from the y-intercepts, microstrain was estimated (Fig. 8).The estimated crystallite size synthesized HAp is shown in Table 2.

Function group analysis
The functional group in the synthesized product is analyzed by Fourier Transform Infrared (FTIR) spectra (Model: IR-Prestige 21 (Shimadzu, Japan)), which are shown in Fig. 9.In HAp, PO 4 3− and OH − are optically active groups, which are responsible for the resulting spectra. 44In this present study, pure and doped HAp were synthesized through the wet chemical precipitation method to modify the crystalline structure, which also shows similar spectra.PO 4 3− (Tetrahedral) ions possess four preliminary forms of vibrations, which are symmetric stretching (n 1 ), asymmetric stretching (n 3 ), symmetric bending (n 2 ), and asymmetric bending (n 4 ). 45Three forms of stretching oscillation were found around 962, 1026, and 1087 cm −1 wavenumbers, whereas bending vibration yielded peaks near 465, 563, and 599 cm −1 wavenumbers, which are equivalent to hydroxyapatite and the results have already been published. 46,47The peak at 962 cm −1 was observed due to (n 1 ) oscillation.Conversely, the peaks at  1087 and 1026 cm −1 were responsible for (n 3 ) vibration.At 563 and 599 cm −1 wavenumbers, (n 4 ) vibrations are observed, while at 473 cm −1 (n 2 ) vibration is predominant.Asymmetric bending (n 4 ) vibration is shown at 563 and 599 cm −1 wavenumbers, while symmetric bending (n 2 ) is observed at 473 cm −1 wavenumbers.In this experiment for synthesized HAp, OH − shows FTIR peaks at 3000-3800 cm −1 wavenumber; these identical positions were reported in numerous literature. 48,49

.3 Optical properties
The spectral band gap of pure and doped HAp was evaluated utilizing a double-beam UV-vis spectrophotometer (Model: U-2910), wherein the powder sample was dispersed in water at room temperature.The absorption frequency of synthesized HAp is used to measure the optical band gap in the UV-vis spectrophotometer.For direct band gap analysis, the Tauc plot method was used, which is expressed in the mathematical eqn (24). 50,51m = A(hq where, h is Planck's constant, E g is the optical band gap.A is a constant, a is the absorption coefficient, m is the photon frequency, as well as n = 1/2 for a direct band gap.The optical band gaps of the synthesized samples were estimated (Fig. 10) and grouped in Table 3.

Scanning electron microscopy (SEM)
The SEM images (Machine model: JEOL JSM-7610F) of synthesized HAp are shown in Fig. 11, where different types of dopants, as well as different precursors, are used for nanocrystalline HAp synthesis.From analyzing the images, it's prominently visible that many distinctive forms of nanoparticles are present in synthesized HAp, which tend to agglomerate.Apart from that, most of these particles are greater than a hundred nanometers as a prominent form.The presence of doped metal oxide was conrmed by the EDS analysis which is visualized in Fig. 11.The existences of Ti and Zn were found in the doped hydroxyapatite.
3.5 Pure and synthesize HAp photocatalytic activity 3.5.1 Effect of contact time on CR degradation.In this experiment, distinctive time frames such as (30, 60, 90, 120, and 150 min) and different amounts of adsorbent like 0.05 g, 0.075 g, 0.1 g, 0.15 g, 0.2 g were observed to estimate the degradation percentage as well as the capacity of CR solution (Fig. 12 and 13).The degradation percentage rises with the increase in adsorbent, as the number of active sites increases, hence boosting the effectiveness of the photocatalyst.The    Similarly, the degradation capacity of the synthesized HAp is investigated for adsorbent 0.05 g, 0.075 g, 0.1 g, 0.15 g, and 0.2 g correspondingly.The optimum degradation capacity is considered for adsorbent 0.1 g and the contact time 90 minutes which are 7.19 mg g −1 , 7.34 mg g −1 , 7.32 mg g −1 , 6.92 mg g −1 for Ca(OH) 2 _HAp, TiO 2 _HAp, CaCO 3 _HAp, and ZnO_HAp, respectively.
3.5.2Effect of catalyst dose on the photodegradation.To investigate the impact of catalytic dose on the photodegradation of CR, several compounds such as Ca(OH) 2 _HAp, TiO 2 _HAp, CaCO 3 _HAp, and ZnO_HAp catalyst from 1.25 to 5 g L −1 at an initial concentration of CR as 2.87 × 10 −5 M as well as irradiation time 90 minutes were employed.Fig. 14 denotes the alteration in the photodegradation of CR as the catalyst at several dosages of the above-mentioned samples.In the case of Ca(OH) 2 _HAp, TiO 2 _HAp, and CaCO 3 _HAp, the observed % of removal of CR is vindicated to rise within catalyst dosage up to 2.5 g L −1 and extended their height values as 89.89%, 91.76% and 91.58% correspondingly.This phenomenon can be ascribed to an increased formation in accessible surface area for the photocatalysts, facilitating the generation of more active radicals. 28,52,53Conversely, with the additional enhancement in the dosage of the catalyst from 2.5 to 5 g L −1 , the percentage of degradation efficacy was attenuated.However, this could be attributed to the high amount of catalytic dose, which makes the solution turbid and reduces the photodegradation of the solution. 54,55Additionally, for ZnO_HAp, the degradation percentage rises with the increase in catalyst dosage, which is around 90% for 5 g L −1 .
3.5.3Effect of solution pH the photodegradation.A group of investigations was accomplished to investigate the effect of pH on the degradation percentage and degradation capacity of CR dye.Different pH, such as pH 5, pH 7, and pH 9 were studied to determine the effect of varying pH (Fig. 15).A 40 mL solution of 20 mg L −1 concentration of CR dye was irradiated at ambient temperature under a 500 W halogen lamp for 90 minutes.The pH of the reaction solution substantially inuences photocatalytic degradation, as it effectively streamlines the entire process.However, estimating the effect of solution pH on photodegradation is a crucial event; several variables have been identied affecting this, such as the electrostatic and catalyst's nature and the presence of the pollutant molecule. 56,57Lower pH levels are observed to increase the photodegradation of weakly acidic contaminants, contradicting previous study results. 58,59he value of degradation percentage increased with increasing   pH from 5 to 7 but decreased at pH 9. The reaction was greatly impacted by the numerous hydroxyl and hydrogen ions, resulting in a larger expenditure owing to the requirement for more effort and an acidic solution; hence, pH 7 was picked as the optimal value.
3.5.4Effect of initial CR concentration on photodegradation.The concentration of pollutants possesses a crucial role in photocatalytic degradation, and investigations were done to establish the appropriate dye concentration for optimal effects.For pH 7 and 2.5 g L −1 of catalyst dose, the impact of various dye concentrations was analyzed.In Fig. 16, the percentage of degradation as well as degradation capacity are denoted.From the analysis, it's unequivocally stated that the degradation percentage increases within the dye concentration raised from 10 mg L −1 to 40 mg L −1 , which can be correlated to the manner that the extent of a suitable number of active sites as well as the radicals are present on the synthesized HAps surface.Furthermore, the additional expansion in initial dye concentration above 40 mg L −1 results in a decrease in the efficacy of degradation percentage.The removal of CR dye diminishes with increasing dye concentration owing to the capture of more photons by the dye compared to the photocatalyst, which produces a low amount of hydroxyl radicals. 60he number of active sites produces more active radicals O 2 c − as well as cOH, which maximize the efficiency of photocatalytic event.Conversely, the reduction in the degradation percentage are observed when the number of free radicals becomes low.In comparison to the degradation percentage, the degradation capacity increased by increasing the concentration of the dye solution.
3.5.5Photocatalytic mechanism of HAp.The photodegradation technique employs a photon source to activate a redox reaction, enhancing the efficacy of the process by limiting recombining properties. 51The proposed simplied reaction mechanism for Congo red degradation using pure, TiO 2 as well as ZnO doped HAp is illustrated in Fig. 17 and mathematically expressed in eqn ( 25)- (32).
Doping hydroxyapatite (HAp) with materials like TiO 2 and ZnO alters its electronic and optical properties, particularly its band gap, enhancing photocatalytic activity.This process creates defects and vacancies in the HAp lattice, facilitating electron-hole pair separation and improving reaction efficiency.The effect of doping on HAp's band gap and photocatalytic activity is complex and depends on factors like dopant type, concentration, synthesis method, and application.Direct band gap materials are preferred due to their prolonged lifetime of charge carriers, while indirect band gap materials may have advantages, but their direct band gap is inherent to HAp. [61][62][63][64] Photocatalytic agents, such as free radicals and electrons, play a crucial part in the photocatalytic deterioration of Congo red dye.These agents, coupled with holes, act as effective oxidizing agents, helping in the formation of more reactive species owing to the delayed reproduction of e − as well as h + .This phenomenon can be mathematically expressed with the help of Mulliken's theory eqn (33) and (34). 65 In these equations, E CB (energy of conduction band), X (electronegativity of the photocatalyst), E c (free electron energy and its magnitude is 4.5 eV), E bg (band gap energy), and E VB (valence band energy), correspondingly.Synthesized HAp possesses electronegativity as 5.89 eV, which is attributable to the geometrical mean of its structure, depicted in literature. 65The estimated magnitude of the conduction band, as well as the valence band, are shown in  The dye solution was ltered and dried at 60 °C in an oven for 2 hours, and then the new solution of CR dye was introduced to the dried samples.From Fig. 18, it's prominently visible that the degradation percentage for the rst cycle, Ca(OH) 2 _HAp, and ZnO_HAp, shows a lower degradation percentage as compared to TiO 2 _HAp as well as CaCO 3 _HAp.In the second cycle, ZnO_HAp exhibited a cabalistic decrease in degradation, while CaCO 3 _HAp depicted the lowest degradation percentage.Finally, in the third cycle, CaCO 3 _HAp and ZnO_HAp had lower percentages of degradation as compared to the Ca(OH) 2 _HAp and TiO 2 _HAp, whereas Ca(OH) 2 _HAp showed lower degradation.This phenomenon of adsorption of dye molecules on the photocatalyst surface can be described as the extent of unoccupied active sites present in the photocatalyst.A greater amount of photodegradation efficiency is observed where the dye molecules are easily adsorbed by active sites staying in the samples.Since the quantity of active sites gets more engrossed within the cycles, this causes lower photocatalytic degradation in the subsequent cycle.
3.5.7 Scavenging studies.2-Propanol (IPA) and EDTA were used as the scavenging agents for OH* and electrons correspondingly.Fig. 19 shows a scavenging test that depicts 2propanol and EDTA, considerably decreased degradation rate, indicating the OH* and electrons are preliminary photoactive species related to photodegradation of CR dye.Conversely, in both scavenging tests, TiO 2 _HAp shows a different phenomenon where degradation percentage increased while adding IPA as well as EDTA, which can be the reason for having holes as a predominant.

Kinetics study
The photodegradation kinetics (Fig. 20) of CR by Ca(OH) 2 _Hap, TiO 2 _Hap, CaCO 3 _Hap, and ZnO_Hap have been studied under simulated sunlight.7][68][69] The degradation rate of dyes may be stated as: where, C 0 = initial concentration of reactant (mol L −1 ), and C = nal concentration of reactant (mol L −1 ).The rst-order rate constant (K 1 ) was estimated by plotting time (t) along the x-axis and −ln(C/C 0 ) along the y-axis, and generated graph is shown in Fig. 20.Table 5 provides a detailed record of the rate constant (k 1 ) and regression coefficient (R 2 ).The research data reveals a correlation between the reaction rate and the catalyst composition.The rst-order rate constant values range from 0.82636 min −1 (ZnO_HAp) to 1.46661 min −1 (Ca(OH) 2 _HAp), with an average of 1.172755 min −1 .The lower rate constant indicates a slower reaction compared to pure HAp, while a higher rate constant indicates a faster reaction.[72]

Practical applications of this research
The laboratory scale study analyzed hazardous compounds in industrial wastewater, highlighting the need for further data on treating real-world wastewater containing a blend of organic and inorganic compounds.This study can be replicated using various pollutant types, including caprolactam, phenol, benzoic acid, toluene, adipic acid, anionic and cationic dyes, benzene, amoxicillin, and ciprooxacin, but requires extensive literature study and a pilot plant study before industrial application.

Conclusion
Hydroxyapatite (HAp) was synthesized successfully in pure and metal-oxide-doped form and crystallite size, calculated from various models, carried good evidence for the formation of nano-sized products.The effectiveness of these synthesized materials as potential photocatalysts was evaluated, with factors such as contact time, catalyst dose, initial dye concentration, pH, radical scavengers, and catalyst reusability inuencing activity, and found these materials can be applied as potential photo-catalysts for degradation of organic pollutants.The synthesized products maintained excellent catalytic activity even aer three reuse cycles.TiO 2 -doped HAp showed 90% degradation of Congo red dye, suggesting it could be a potential candidate for synthetic dye degradation compared to pure and ZnO-doped HAp.It may also be applied for the degradation of growing contaminants in pharmaceutical wastewater, which is composed of most antibiotics.Overall, TiO 2 -doped HAp has signicant potential in photocatalysis applications, and further research can be performed for industrial scale application.

Fig. 1
Fig.1Systematic approach for pure and metal-oxide doped HAp synthesis.

Fig. 2
Fig. 2 Laboratory setup for investigating photodegradation with halogen lamp.

Fig. 3
Fig. 3 XRD patterns of pure and doped HAp (A) full scan, (B) focused region.

42 ,43 b hkl 2 = 2 ( 20 )
b L b hkl + b G where, b L = FWHM for Lorentzian function.b G = FWHM for Gaussian function.The approach lends a larger weight to Bragg peaks in small and intermediate angles, decreases reection overlapping, and connects crystallite size and lattice 3 with the H-W technique, as indicated by eqn (21)-(23).34

Fig. 14
Fig. 14 Effect of various doses on the photodegradation (A) degradation percentage and (B) degradation capacity.

Fig. 15
Fig. 15 Impact of pH on photodegradation (A) degradation percentage and (B) degradation capacity.

Fig. 18 .
Denotes the recyclability test of synthesized pure and dope HAp at optimum parameters like 0.1 g of catalyst, 2.87 × 10 −5 M, 40 mL CR solution, at 90 minutes under halogen lamp (500 W) for three cycle tests.

Fig. 18
Fig. 18 Reusability of synthesized HAp in terms of degradation percentage.

Fig. 20
Fig.20The plot of −ln(C/C 0 ) against time (min) for various samples to estimate the reaction rate constant for 0.1 g of photocatalyst.

Table 3
Estimated band gap of pure and synthesized HAp

Table 4 .
28e Synthesized HAp demonstrated greater negativity potentials of the Conduction band than O 2 /cO 2 − (−0.33 eV) as well as greater positive potentials of the valence band compared to OH/cOH (1.99 eV), showing both radicals can be generated for photocatalysis of the Congo red dye.3.5.6Photocatalytic reusability experiments.The recyclability or reusability test is a vital criterion that measures a catalyst's optimum and repeated usage, assuring its long-term sustainability.28

Table 4
Synthesized HAp Valance Band (VB) as well as Conduction Band (CB) potentials for

Table 5
Estimated values of linear fit for synthesized HAp of 0.1 g photo catalyst dose